advertisement

International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net Optimization of Aggregate Gradation and its effects on properties of normal strength concrete(M20) Adapala Kalpana1, Ravuru Neelavathi2 and Dr K.Narasimhulu3 1,2,3Department of Civil Engineering, Annamacharya Institute of Technology and Sciences, Tirupati, India ---------------------------------------------------------------------***---------------------------------------------------------------------- Abstract - Aggregate as the main constituent of concrete about 70.0% to 80.0 % occupy the total volume of the concrete. They highly affect the both fresh and hardened concrete properties of the concrete. By using the optimization techniques such as Talbot’s grading curve or Power curve, Coarseness factor chart and Fineness modulus. The cement content can be reduced, it gives the dense arrangement and improve the properties of the concrete such as workability, durability, compressive strength, etc., from this experimental investigation by using of this optimization of combined aggregate gradation the concrete is prepared by using the different N values are 0.45,0.55,0.65 and 0.75 based on the fineness modulus. In this experimental investigation the mix design is done for Normal strength concrete of 20MPa based on IS 10262:2009 and optimization techniques and prepared specimen. The tests are conducted on fresh and hardened concrete like Slump test, Bulk density of concrete, Compressive strength, Rebound hammer, Ultrasonic pulse velocity and water absorption test. Based on the test results the N value is 0.45 for maximum compressive strength and high workability. Cement content can be reduced up to 15% is possible for 20Mpa normal strength concrete based on the test results. Key Words: Coarseness factor, Workability factor, Power Curve, Fineness modulus, Slump, Compressive strength 1. INTRODUCTION In concrete the main constituents are cement, water, aggregates. In cement concrete the aggregates are occupy nearly 70% to 80% of the volume concrete. Normally aggregates is the important constituents in the concrete. It gives as structure of the concrete. The aggregates effects on the properties of fresh and hardened concrete. The aggregates reduce the shrinkage and economy of the concrete. By use of the aggregates their influence on cement concrete properties like strength, durability workability etc. For the achievement of high economy, the aggregates should be made clean, strong, bond strength, shape and texture, specific gravity, bulk density, voids, moisture content, fineness modulus and porosity. The concrete mix preparation made by using of cement, coarse aggregates of two different sizes such as 20mm, 10mm, fine aggregate and potable water used for mixing. The coarse aggregates give the good structural ability to the concrete and fine aggregates fill the gaps between the coarse aggregates, remaining gaps in fine aggregates fills by the cement paste. The used coarse aggregates also increasing the bulk density of the concrete. Normally from production of the concrete, cement is the most expensive material about 55% to 60% of the total cost of the production of concrete material. The paste content only 25% to 35% of the total volume of the concrete. The properties of the concrete can be improved by using well graded aggregates, the well gradation in aggregate can be attained by optimization of aggregate gradation in these views the importance of optimization of the aggregate is arises. The most suitable of aggregates gradation for concrete mix, however will depends up on actual grading, particle sizes and surface texture. The optimization of aggregate grading is the most advantage technique for economical and technical reasons. By using of this optimization combined gradation of aggregates mixing cement content is reduced up to 10% to15% of the total volume of the concrete and durability of concrete increased by decreasing the permeability, decreasing drying shrinkage and cracking of the concrete. By increasing the volume of aggregates in total volume of concrete porosity and voids will be decreased it will lead to increasing the structural performance of concrete. The optimization of the combined aggregate gradation provides the densest arrangement of aggregates in given volume of concrete, it also decreases the volume of cement paste required for sufficient workability. The optimization results to improve in the workability, finish ability, pumpability and reduced segregation, when compare to the concrete poorly graded aggregate gradation. It also reduced the shrinkage was directly reducing the cement paste in cement concrete with possible of the increasing the aggregate content in concrete and reduced the shrinkage translates into reduced concrete. 2. LITERATURE REVIEW The Fuller and Thompson has given groundbreaking work on optimization gradation to the concrete on greatest strength and workability. They concluded to attain high density, aggregates should be well graded in sizes and combined with cement paste. An ideal maximum density curve was developed. The maximum density achieved was mainly due to the greatest density of the © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 1456 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net aggregates only and not necessarily the greatest density when combined with the cement paste because of the way the cement particles fit into the smaller pore (Fuller and Thompson 1907). The idea that aggregate gradation could be controlled and thus affect concrete properties led to other research and ultimately to specification governing aggregate gradation. Wig et al. suggested that Fuller and Thompson’s conclusions could not necessarily be extrapolated to aggregate different from the ones used in the original study. It was shown that the Fuller curve may not always give the maximum strength or maximum density (Wig et al. 1916). Their work indicated that for a given maximum particle size, D, the equation produces the maximum density when n=0.5. It concluded that aggregate so graded would produce concrete mixture that will be harsh and difficult to place and were not really usable (Talbot and Richart 1923). Other authors are in agreement with conclusion, and eventually maximum density proportioning method fell out of favor (McMillian 1929; Walh 1933; Besson 1935; Blanks et al 1940; Frost 1967) Shilstone in 1970, found several factors on concrete properties depends on the aggregate gradation. A methodology was developed for well graded aggregates which includes the fine aggregate, intermediate aggregate and coarse aggregate particle sizes. Coarseness factor chart was developed in 1990, which identifies the individual size percent retained in excessive or in deficient. (Shilstone 1970). 3. PROPERTIES OF MATERIAL AND METHODOLOGY The physical properties of all the materials used in the present experimental investigation on cement, fine aggregate, coarse aggregate based on the standard experimental procedures as per IS code provisions. The experimental work conducted are Sieve Analysis, Specific gravity, crushing value, impact value, water absorption, shape test (flakiness and elongation), LosAngeles abrasion, bulk density on coarse aggregate and fine aggregate and bulking of fine aggregate tests. Concrete Mix design was designed using the optimization techniques and IS10262:2009. Three concrete mixes were prepared with three different sands based on the fineness modulus and conducted destructive test for Compressive Strength. 4. MATERIALS Cement is a good substance which acts as a binding agent for materials like sand, coarse aggregate and water. In this experimental investigation the Ultra Tech cement of PPC cement was used. The coarse aggregate sused are 20 mm and 12.5 mm crushed aggregates. The coarse aggregate was taken from Chandragiri quarry near Chandragiri Kota Chittoor (Dist), Andhra Pradesh. The physical properties of the coarse aggregate are shown Table: 1 The fine aggregates used are river sand which was from Swarnamukhi river banks near Sri Kalahasthi, Chittoor (Dist), Andhra Pradesh. The river sand used are classified into coarse, medium and fine depending upon the grain size. The physical properties of the river sand are shown Table 2. Further, the portable water was used for mixing and curing. Table: 4.1 Physical Properties of Cement S.NO Particulars Cement 1 Normal Consistency 32 % 2 Fineness of cement 6% 3 Specific gravity of cement 3.10 Table: 4.2 Physical Properties of Coarse Aggregate S. No 1 2 3 4 5 6 7 © 2019, IRJET | Particulars Crushing value Impact value Los angel’sabrasion test on coarse aggregate Shape test Flakiness index Elongation index Bulk density Bulk density of aggregate Specific gravity Water absorption Impact Factor value: 7.34 | Coarse aggregate 24.16% 16.80% 27.41% 12.87 % 12.86 % 14.81 KN/ m³ 2.65 0.5% ISO 9001:2008 Certified Journal | Page 1457 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net Table: 4.3 Physical Properties of Sand S.No Particulars Sand 1 Specific gravity 2.66 2 Bulk density 16.35 KN/m³ 3 Water absorption 1.2 % 5. METHODOLOGY In this experimental investigation are used in the optimization of aggregate gradation such as Talbot’s grading curve or power curve, coarseness factor chart and fineness modulus and also IS 10262:2009 prepared six concrete mix designs normal strength concrete of 20 MPa on based on the physical properties of the materials. The six concrete mixes are prepared by using different in N value 0.45,0.55,0.65 and 0.75 are calculated mix proportions. Themix prepared with cement, coarse aggregates, fine aggregates and water. The proportion of the volume of aggregates in concrete (Coarse and Fine) are not fixed based on the Zone confirming. Based on the optimization of combined aggregate gradation technique of power curve fixing the trail proportions to the volume of the concrete. The well grade concrete is prepared based on the coarseness factor chart. MIX DESIGN The mix design is designed based on Absolute volume method, the volume of the aggregate proportions is taken by trail, by optimization technique of Power curve. The Table shows the values of proportioning and material test data. Table 5.1 Mix Design Proportioning Specifications For Proportioning Grade of designation Type of cement Max. size of the aggregate Min. cement content M20 PPC 20 mm 322 Kg/m3 Max. cement content 450 Kg/m3 Max. water cement ratio Exposure condition Method of concrete placing Type of the aggregates 0.59 Severe (for reinforced concrete) Pumping Crushed angular aggregates Table 5.2 Specific gravity and Water absorption values for Aggregates Sp. Gravity Cement water Coarse Aggregates Fine Aggregates 3.1 1 2.65 2.65 0.50% 1.20% Water Absorption © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 1458 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net Table: 5.3 Combined Aggregate Grading Analysis for Aggregate Proportion Combined passing (%) Combined retaining (%) Individual retaining (%) 0.45 Power curve 100 100 100 0.00 0.00 100 2 20 89.25 100 100 98.20 11.80 1.80 86.5 3 16 36.27 100 100 89.29 10.71 8.91 74.8 4 12.5 5.42 83.53 100 77.88 22.12 1.41 63.7 5 10 0.78 32.51 100 57.51 42.49 2.37 55.1 6 4.75 0 1.39 100 54.72 55.28 12.80 34.0 7 2.36 0 0.15 92.3 41.40 58.50 3.22 21.6 8 1.18 0 0.12 76.6 34.44 65.56 7.06 13.5 9 0.6 0 0 48.1 22.05 77.95 12.39 8.9 10 0.3 0 0 13.2 5.93 94.07 16.12 5.6 11 0.15 0 0 2.9 1.30 98.70 4.62 3.6 Combined Fineness Modulus of CA 72.63 Workability factor Aggregate 2 10 mm 100 Coarseness factor Aggregate 1 20 mm 25 4.75 mm Sieve Size (mm) 1 Aggregate 3 S. No (0.167:0.384:0.45) for N = 0.45(0) 41.50 5.3 % COMBINED PASSING 0.45 POWER CURVE COMBINED PASSING (%) 120.00 100.00 80.00 60.00 40.00 20.00 0.00 0.1 1 10 100 SIEVE SIZE (mm) Figure: 5.1 Combined Passing with 0.45 Power Curve for Aggregate © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 1459 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net Proportion (0.167:0.384:0.449) Figure: 5.2 The coarseness Factor Chart for N = 0.45,0.55,0.65,0.75(300). 6. MIX PROPORTIONS The mix percentages of aggregate are given in Table: 6 and mix proportions of the material are given in Table: 6 Table: 6.1Mix Proportions with different N values % of Sand Cement Kg/m³ Water Kg/m³ 20 mm Aggregate Kg/m³ 10 mm Aggregate Kg/m³ Fine Aggregate Kg/m³ Total 45% 322.03 190 361.05 655.40 833.55 2362 0.59 41% 322.03 190 385.95 700.60 763.45 2362 0.65 0.59 37% 322.03 190 410.85 745.80 693.35 2362 M4 0.45 0.59 45% 322.03 190 308.95 710.40 830.65 2362 M5 0.55 0.59 47% 322.03 190 320.85 663.40 865.75 0.59 37% 322.03 190 454.15 703.70 692.15 Mixes N Values M1 0.65 W/C Ratios 0.59 M2 0.65 M3 M6 0.75 2362 2362 7. TESTS CONDUCTED In this experiment we study the concrete prepared by different N values0.65, 0.45,0.55 and 0.75.The different sand percentages are 45%, 41%, 37%,45%, 47% and 37%for all the six mixes of the concrete but different N values are taken 0.65,0.45,0.55 and 0.75. The N value 0.65 are different ratios of the increases the sand improves good workability of the concrete. The sand taken 200,300 and 400 kg’s are added to the mix because the workability can be improved this N values 0.65 and the remaining N values are 0.55, 0.75 are sand added only 300 kgs and can be improve the good workability of the concrete. The N values 0.45 are not added to the increase of the sand but its standard values. In this experimental work the tests may be conducted slump test, bulk density of concrete, destructive and non-destructive tests. The destructive test is conducted by compressive strength on prepared by concrete by using the standard cubes of a dimensions are 15 cm × 15 cm × 15 cm and the volume of the cube is 3375 cm3 according to IS codes. The nondestructive tests conducted by Rebound hammer and ultrasonic pulse velocity, water absorption on cubes. 8. RESULTS AND DISCUSSIONS The tests results and the test conducted on fresh concrete and hardened concrete. The tests conducted on fresh concrete are slump test and bulk density of concrete and the tests conducted on hardened concrete are destructive test and © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 1460 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net nondestructive tests, such as Rebound hammer, compressive strength, ultrasonic pulse velocity, water absorption tests are respectively. 8.1 SLUMP TEST In this experimental to study the slump test on conducted for fresh concrete by using the slump cone for all the six concrete mixes. The respective values of the slump with percentages of the sand are 45%, 41%, 37%,45%, 47% and 37%for all the six mixes of the concrete but different N values are taken 0.65,0.45,0.55 and 0.75. The N value 0.65 are different ratios of the increases the sand can be improve good workability of the concrete. The sand taken 200,300 and 400 kg’s are added to the mix because the workability can be improved this N values 0.65 and the remaining N values are 0.55, 0.75 are sand added only 300 kg’s and can be improve the good workability of the concrete. The N values 0.45 are not added to the increase of the sand but its standard values. Table: 8.1 Slump test for different N values S.No 1 2 3 4 N Values 0.45(0) 0.65(200) 0.65(300) 0.65(400) Sand (%) 45.00 37.47 41.26 45.00 Slump(mm) 25 190 150 110 Table: 8.2 Slump test for different N values S.No 1 2 3 4 N Values 0.45(0) 0.55(300) 0.65(300) 0.75(300) Sand (%) 45.00 46.8 41.26 37.47 Slump(mm) 25 15 150 130 8.2 BULK DENITY OF CONCRETE In this experiment we study about bulk density of the concrete test conducted for fresh concrete by using the 3 lit of cylinder for all the six concrete mixes. The Table: 8.3 and Table: 8.4, shows the respective values of the bulk density of the concrete. Table: 8.3 Bulk density of concrete for Different N values SNo 1 2 3 4 N Values 0.45(0) 0.65(200) 0.65(300) 0.65(400) Sand (%) 45.00 37.47 41.26 45.00 Bulk Density(KG/lit) 2.587 2.608 2.559 2.419 Table: 8.4 Bulk density of concrete for DifferentN values SNo 1 2 3 4 NValues 0.45(0) 0.55(300) 0.65(300) 0.75(300) Sand (%) 45.00 46.8 41.26 37.47 Bulk Density(KG/lit) 2.587 2.563 2.559 2.568 8.3 COMPRESSIVE STRENGTH In this experiment we study about the compressive strength test conducted for hardened concrete on the cubes by using the compressive machine of 2000 KN. The cubes are prepared based on the mix design and the test is conducted under curing period of 7 days and 28 days test on cubes. © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 1461 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net Figure: 8.1 combined values for 7 Days and 28 Days Compressive Strength for different N value are 0.65 (37.74,41.26 and 45.00) and 0.45(0) Figure: 8.2 .combined values for 7 Days and 28 Days Compressive Strength for different N value are 0.75(37.47),0.65(41.26),0.55(46.8) and 0.45(45.00) 8.4 REBOUND HAMMER Rebound hammer is the one of the nondestructive tests on the hardened concrete. In this experimental to be study on the test is conducted on a specimen with a curing period of 7 days and 28 days for all the six mixes by using the rebound hammer. Table: 8.5 Combined values of Rebound Hammer Numbers for 7 Days and 28 Days Compressive Strength with Different Percentage of Sand SNo 1 2 3 1 © 2019, IRJET | N Values 0.45(0) 0.65(200) 0.65(300) 0.65(400) Sand (%) 45.00 37.47 41.26 45.00 7 Days Rebound Hammer 20.4 24.0 25.4 22.1 Impact Factor value: 7.34 | 28 Days Rebound Hammer 27.0 26.0 28.9 21.9 ISO 9001:2008 Certified Journal | Page 1462 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net Table: 8.6 Combined values of Rebound Hammer Numbers for 7 Days and 28 Days Compressive Strength with Different Percentage of Sand SNo N Values Sand (%) 1 2 3 4 0.45(0) 0.55(300) 0.65(300) 0.75(300) 45.00 46.8 41.26 37.47 7 Days Rebound Hammer 20.4 23.8 25.4 23.78 28 Days Rebound Hammer 27.0 25.1 28.9 27.3 8.5 ULTRASONIC PULSE VELOCITY Ultrasonic pulse velocity is the one of the nondestructive tests on the hardened concrete. In this experimental to be study on the test is conducted on the specimens with a curing period of 7 day and 28 days for all the six mixes. Table: 8.7 Ultrasonic Pulse Velocities for 7 Days and 28 Days Compressive Strengths with Different N Values SNo N Values Sand (%) 1 2 3 4 0.45(0) 0.65(200) 0.65(300) 0.65(400) 45.00 37.47 41.26 45.00 7 Days Compressive strength(N/mm²) 22 21 21 20 7 Days UPV (m/s) 4392 4286 4273 4316 28 Days Compressive strength(N/mm²) 29 31.5 31.4 22.5 28 Days UPV (m/s) 4702 4725 4703 4634 Table: 8.8 Ultrasonic Pulse Velocities for 7 Days and 28 Days Compressive Strengths with Different N Values SNo N Values Sand (%) 7 Days Compressive strength(N/mm²) 7 Days (m/s) 1 2 3 4 0.45(0) 0.55(300) 0.65(300) 0.75(300) 45.00 46.8 41.26 37.47 22 19 21 16 4392 4209 4273 4209 UPV 28 Days Compressive strength(N/mm²) 29 22 31.4 18 28 Days (m/s) UPV 4702 4616 4703 4583 8.6 WATERABSORPTION TEST The water absorption test can be conducted on the specimens with a curing period of 7 day and 28 days for all the six mixes. The experimentally to be study the normal strength of the concrete cubes are prepared all six mixes in the test are conducted to the water absorption after the 28 days of curing period of concrete cubes. Table: 8.9 Water absorption for after 28 Days with different N Values SNo 1 2 3 4 © 2019, IRJET | N Values 0.45(0) 0.65(200) 0.65(300) 0.65(400) Impact Factor value: 7.34 Sand (%) 45.00 37.47 41.26 45.00 | After 28 Days water absorption (%) 1.88 1.71 1.85 1.98 ISO 9001:2008 Certified Journal | Page 1463 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net Table: 8.10 Water absorption for after 28 Days with different N Values SNo N Values Sand (%) After 28 Days water absorption (%) 1 0.45(0) 45.00 1.88 2 0.55(300) 46.80 2.05 3 0.65(300) 41.26 1.85 4 0.75(300) 37.47 0.46 9. CONCLUSIONS The following conclusions are drawn based on the results obtained from the tests. 1. Based on the testsresults the compressive strength gained more than the target strength of the concrete for different fineness modulus of the sands and different n values like0.65,0.45,0.55 and 0.75. 2. The n value 0.65 of the compressive strength for 5.3 fineness modulus and percentages of 45% of sand are 22.5 N/mm2respectively. 3. The n value 0.65 of the compressive strength for 5.5 fineness modulus and percentages of 41% of sand are 31.4 N/mm2respectively. 4. The n value 0.65 of the compressive strength for 5.7 fineness modulus and percentages of 37% of sand are 31.5N/mm2respectively. 5. The n value 0.45 of the compressive strength for 5.3 fineness modulus and percentages of 45% of sand are 29 N/mm2respectively. 6. The n value 0.55 of the compressive strength for 5.2 fineness modulus and percentages of 47% of sand are 22 N/mm2respectively. 7. The n value 0.75 of the compressive strength for 5.7 fineness modulus and percentages of 47% of sand are 20.6 N/mm2respectively. 8. The maximum compressive strength, Slump, Bulk density, Rebound hammer number, water absorption and UPV are obtained with 45 % of the Sands for n value 0.65. 9. The maximum compressive strength, Slump, Bulk density, Rebound hammer number, water absorption and UPV are obtained with 41 % of the Sands for n value 0.65. 10. The maximum compressive strength, Slump, Bulk density, Rebound hammer number, water absorption and UPV are obtained with 37 % of the Sands for n value 0.65. 11. The maximum compressive strength, Slump, Bulk density, Rebound hammer number, water absorption and UPV are obtained with 45 % of the Sands for n value 0.45. 12. The maximum compressive strength, Slump, Bulk density, Rebound hammer number, water absorption and UPV are obtained with 47 % of the Sands for n value 0.55. 13. The maximum compressive strength, Slump, Bulk density, Rebound hammer number, water absorption and UPV are obtained with 37 % of the Sands for n value 0.75. REFERENCES 1. Shiltone, J.M (1989). “A Hard Look at concrete.” Civil Engineering: 47-49. 2. Shilstone, J.M (1990). “Concrete Mixture Optimization.” Concrete International 12(6):33-39. 3. Shilstone, J.M. (1990). Mixture Optimization for Fast-Track. 69thannual Transportation Research Board meeting, wahington, D.CA © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 1464 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 07 | July 2019 p-ISSN: 2395-0072 www.irjet.net 4. Talbot and F.E Richart(1923).“The Strength Concrete and its Relation to The Cement, Aggregate and Water.” Bulletin No 137:1-116. 5. Taylor, M.A. (1986). “Concrete Mix Proportioning by Modified Fineness Modulus Method.” Concrete International: 4752. 6. Washingtone DOT (2004). “Combined Aggregate Gradation for Portland Ceement Concrete, Standard Specifications, Section 9-03.1(5)”1. 7. Wilson,P. and D.N. Richardson (2001). “Aggregate Optimization of Concrete Mixtures.”Rolla, Missouri, University of Missouri-Rolla:18. 8. S.D. Baker, C.F. Scholar, (1973). “Effect of Variations in Coarse-aggregate Gradation on properties of Portland Cement Concrete.” Highway Research Board, Issue No 441. 9. Sandor Popovics, (1973) “ Aggregate Grading and the Internal Structure Of Concrete” Highway Research Board, Issue No 441 10. S.B. Hudson, H.F. Waller, (1969) “Evaluation of Construction Control Procedures: Aggregate Gradation Variations and Effects.” NCHRP Report, Issue No. 69, Publisher- Transportation research Board. 11. Shu-T‟ien Li, V. Ramakrishnan, 1973. “Gap Graded Aggregates for High Strength Concretes” Highway Research Board, Issue No 441 12. C.P. Marais, E. Otte, L.A. Bloy 1973 “The Effect of Grading on Lean Mix Concrete”. Highway Research Board, Issue No 441 13. Karthik H. Obla and Haejin Kim., (2008), “On Aggregate GradingIs good concrete performance dependent on meeting grading limits” Concrete Iinternational, pp 4550. 14. Harrison, P.J., 2004, For Ideal SlabonGround Mixture, Concrete International, 26(3), pp 4955. 15. Shilstone, J. M. Sr., 2002, Performance based concrete mixtures and specifications for today, Concrete International. 16. W B Ashraf And M A Noor “Performance- Evalution of Concrete Properties for Different Combined Aggregate Gradation” Approaches The Twelfth East Asia- Pacific Conference on Structural Engineering & Construction, Hongkong, (2011) 17. C Mc Call and M E King (2005) on “Effects of Aggregate Grading on Drying Shrinkage of Florida Concretes”, Concrete International 44-45 18. Book- ‘’Concrete Technology’’, Author: M.S. Shetty, S Chand Publications. 19. Book- “Concrete Technology”, Authors: A.M. Neville and J.J. Brooks, Pearson Education, Second Impression 2007. 20. Book- “Concrete Technology”, Author: Gambier. 21. Book- Engineering Materials” Author: Rangwala, Charotarpubicatons. 22. IS 10262:2009, Concrete Mix Proportioning (first revision), Bureau of Indian Standards, New Delhi. 23. IS 383:1970, Specifications for Coarse and Fine Aggregate from Natural Sources for Concrete (second revision), Bureau of Indian Standards, New Delhi. © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 1465